Formation of a molecular spin ladder induced by a supramolecular cation structure
Nishihara, Sadafumi; Akutagawa, Tomoyuki; Hasegawa, Tatsuo; Nakamura, Takayoshi; Chemical Communications  (2002) 408–; doi:10.1039/b110368g

data_7114335
_publ_section_title
;
 Formation of a molecular spin ladder induced by a supramolecular cation
 structure
;
_journal_issue                   5
_journal_name_full               'Chemical Communications'
_journal_page_first              408
_journal_paper_doi               10.1039/b110368g
_journal_year                    2002
_chemical_compound_source        'synthesized by the authors, see text'
_chemical_formula_sum            'C46 H64 N4 Ni2 O12 S20'
_chemical_formula_weight         1623.63
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_audit_creation_date             'Thu Dec 20 18:30:06 2001'
_audit_creation_method           'by teXsan'
_cell_angle_alpha                73.5786(9)
_cell_angle_beta                 76.2712(8)
_cell_angle_gamma                82.426(1)
_cell_formula_units_Z            2
_cell_length_a                   13.1321(4)
_cell_length_b                   16.3032(5)
_cell_length_c                   17.6903(5)
_cell_measurement_reflns_used    26974
_cell_measurement_temperature    296.2
_cell_measurement_theta_max      27.5
_cell_measurement_theta_min      1.5
_cell_volume                     3520.60(18)
_computing_cell_refinement       PROCESS-AUTO
_computing_data_collection       PROCESS-AUTO
_computing_data_reduction        'teXsan Ver. 1.10'
_computing_molecular_graphics    ORTEP-III
_computing_publication_material  'teXsan Ver. 1.10'
_computing_structure_refinement  'teXsan Ver. 1.10'
_computing_structure_solution    SIR92
_diffrn_ambient_temperature      296.2
_diffrn_measurement_device_type  Rigaku
_diffrn_measurement_method       \w-scan
_diffrn_orient_matrix_UB_11      0.00000
_diffrn_orient_matrix_UB_12      0.00000
_diffrn_orient_matrix_UB_13      0.00000
_diffrn_orient_matrix_UB_21      0.00000
_diffrn_orient_matrix_UB_22      0.00000
_diffrn_orient_matrix_UB_23      0.00000
_diffrn_orient_matrix_UB_31      0.00000
_diffrn_orient_matrix_UB_32      0.00000
_diffrn_orient_matrix_UB_33      0.00000
_diffrn_radiation_detector       'Imaging Plate'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.054
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       0
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            55511
_diffrn_reflns_reduction_process 'Lp corrections applied'
_diffrn_reflns_theta_max         27.48
_diffrn_standards_decay_%        0.00
_diffrn_standards_interval_count 0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    1.182
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    1.531
_exptl_crystal_density_meas      ?
_exptl_crystal_description       needle
_exptl_crystal_size_max          0.800
_exptl_crystal_size_mid          0.300
_exptl_crystal_size_min          0.300
_refine_diff_density_max         0.31
_refine_diff_density_min         -0.37
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.109
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     757
_refine_ls_number_reflns         8095
_refine_ls_number_restraints     0
_refine_ls_R_factor_gt           0.0377
_refine_ls_shift/su_max          0.0006
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.0943
_reflns_number_observed          8095
_reflns_number_total             16043
_reflns_observed_criterion       F^2^>3.0\s(F^2^)
_cod_data_source_file            b110368g.txt
_cod_data_source_block           2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_cell_volume        3520.6(2)
_cod_original_sg_symbol_H-M      'P -1         '
_cod_database_code               7114335